1 University of Rome “Tor Vergata” Consiglio Nazionale delle Ricerche
UNIVERSITY OF ROME “TOR VERGATA”
Dr. Vincenzo Baglio
Ph.D. course in “Materials for Environment and Energy”
Preparation and characterization of components for Direct
Methanol Fuel Cells
TABLE OF CONTENTS
I.1 – Introduction to Direct Methanol Fuel Cells pag. 5 I.2 – Fundamental Aspects pag. 6
I.2.1 – Anodic oxidation of methanol pag. 6
I.2.1.1 – Overall reaction pag. 6
I.2.1.2 – Electrocatalysis pag. 7
1.2.1 – General comments pag. 7
1.2.2 – Experimental methods pag. 8
1.2.3 – Structural effects and electrode-kinetics pag. 10
1.2.4 – Pt electrocatalysts pag. 11
1.2.5 – Pt-Ru binary alloy electrocatalysts pag. 13 1.2.6 – Promoting effects of Ru and Sn: bifunctional mechanism
and ligand effect pag. 15
1.2.7 – Role of Ru-oxide in enhancing kinetics pag. 18 1.2.8 – Ternary alloy Pt-Ru-W and Pt-Ru-Mo electrocatalysts pag. 19 1.2.9 – Heteropolyacids as surface promoters pag. 20 1.2.10 – Alternative electrocatalysts to Platinum and their alloys pag. 21 I.2.1.3 – Morphological aspects of electrocatalysts pag. 23 1.3.1 – Role of surface area and metal loading pag. 23
1.3.2 – Role of carbon support pag. 24
1.3.3 – Preparation methods pag. 25
I.2.2 – Cathodic reduction of oxygen pag. 26
2.1 – General considerations pag. 26
2.2 – Oxygen electroreduction in DMFCs pag. 27
2.3 – Carbon supported electrocatalysts pag. 29 2.4 – Non-noble metal based electrocatalysts pag. 31 I.3 – Technology Development and its Prospects pag. 32
I.3.1 – Proton conducting membranes pag. 32
I.3.2 – Membrane and electrode assemblies pag. 34
I.3.3 – Single cell performance – Polarization behaviour pag. 36 3.1 – Dependence on kinetics of electro-oxidation of methanol and
oxygen reduction pag. 36
3.2 – Effect of methanol concentration, pressure and flow rates on
DMFC performance pag. 38
3.3 – Effect of methanol cross-over pag. 39
3.4 – Flow fields pag. 41
I.4 – References pag. 43
CHAPTER II – Catalysts development and characterizationpag. 51 II.1 – Effect of Pt-Ru alloy composition on high-temperature methanol
electro-oxidation pag. 51
II.1.1 – Introduction pag. 51
II.1.2 – Experimental pag. 53
II.1.3 – Results and Discussion pag. 54
3.1 – Physico-chemical analysis pag. 54
3.2 – Electrochemical studies pag. 62
3.3 – Mechanism and kinetic equation pag. 66
II.1.4 Conclusions pag. 67
II.1.5 References pag. 69
II.2 – Analysis of the high temperature methanol oxidation
behaviour at carbon supported Pt-Ru catalysts pag. 72
II.2.1 – Introduction pag. 72
II.2.2 – Experimental pag. 73
II.2.3 – Results and Discussion pag. 75
II.2.4 – References pag. 93
II.3 – Electrochemical analysis of high temperature methanol
electro-oxidation at Pt-decorated Ru catalysts pag. 95
II.3.1 – Introduction pag. 95
II.3.2 – Experimental pag. 96
II.3.3 – Results and Discussion pag. 97
II.3.4 – Conclusions pag. 98
II.3.5 – References pag. 106
CHAPTER III – Membranes development and characterizationpag. 107 III.1 – Influence of the acid base characteristics of inorganic
fillers on the high temperature performance of composite
III.1.1 – Introduction pag. 107
III.1.2 – Experimental pag. 109
III.1.3 – Results and Discussion pag. 111
III.1.4 – Conclusions pag. 132
III.1.5 – References pag. 134
III.2 – Influence of TiO2 nanometric filler on the behaviour of a composite
membrane for applications in direct methanol fuel cells pag. 136
III.2.1 – Introduction pag. 136
III.2.2 – Experimental pag. 136
III.2.3 – Results and Discussion pag. 138
III.2.4 – Conclusions pag. 151
III.2.5 – References pag. 152
III.3 – Zeolite-based composite membranes for high temperature direct
methanol fuel cells pag. 153
III.3.1 – Introduction pag. 153
III.3.2 – Experimental pag. 153
III.3.3 – Results and Discussion pag. 155
III.3.4 – Conclusions pag. 161
III.3.5 – References pag. 162
Direct Methanol Fuel Cells (DMFCs) are becoming an important area of research, due to their potentialities for a wide application in the next future as electrical power generators because of their low environmental impact. The fields in which these devices may find application involve transportation, portable power sources and distributed generation of clean energy. Yet, the commercial application of these devices is limited by the presence of two main drawbacks that have hindered the achievement of high performances: (i) the slow methanol oxidation kinetics and (ii) the methanol cross-over through the perfluorosulfonic membranes commonly used as electrolyte in these systems. Thus, the topics of this PhD thesis, and, consequently, of my research activity, are concerning with:
a) analysis of high temperature methanol electro-oxidation at different Platinum-based catalysts, i. e. unsupported Pt-Ru alloys of various compositions in terms of metal atomic ratio, supported Pt-Ru catalysts varying by different concentrations of metallic phase on carbon support, Pt-decorated Ru catalysts;
b) composite Nafion membranes containing different hygroscopic ceramic oxides for high temperature DMFC operation (130-150°C).
The recent developments in both fundamental and technological aspects of Direct Methanol Fuel Cells are also described and included in Chapter I of this thesis.
The research activity concerning with the development of catalysts for the methanol electro-oxidation reaction and their physico-chemical and electrochemical characterization is reported in Chapter II.
The preparation and characterization of composite perfluorosulfonic membranes based on recast Nafion containing finely dispersed inorganic oxides is reported in Chapter III, togheter with an analysis of the mechanisms governing the conductivity/water retention properties relationship.
I.1 Introduction to Direct Methanol Fuel Cells
Direct methanol fuel cells (DMFCs) working at low and intermediate temperatures (up to 150°C) and employing solid protonic electrolytes have been postulated as suitable systems for power generation in the field of electro-traction [1-6]. DMFCs utilize liquid fuel to deliver a continuos power but they have higher utilization efficiencies and intrinsically lower polluting emissions with respect to internal combustion engines. Since transportation represents a significant portion of world energy consumption and contributes considerably to atmospheric pollution, the development of an appropriate fuel cell system is an important issue from both economical and environmental point of views. In order to be competitive within the transport market, the DMFC must be reasonably cheap and capable of delivering high power densities. At present, there are a few challenging problems in the development of such systems [1-7]. These mainly consist in finding i) electrocatalysts which can effectively enhance the electrode-kinetics of methanol oxidation ii) electrolyte membranes which have high ionic conductivity and low-methanol cross-over and iii) methanol tolerant electrocatalysts with high activity for oxygen reduction. Furthermore, a significant relevance play all the aspects related to fuel cell stack development, in particular, materials and design of cell housing, bipolar plates, gaskets, and stack auxiliaries. All these materials and devices contribute to the final characteristics of practical devices determining the performance, efficiency and cost. At present, the cost of the entire system is mainly determined by the presence of noble metals in the catalyst and the use of Nafion membranes [3-5].
I.2 Fundamental Aspects
I.2.1 Anodic oxidation of methanol
I.2.1.1 Overall reaction
Most of fuel cell systems operate with hydrogen as a fuel. Electro-oxidation of hydrogen is a fast reaction on a low loading Pt electrocatalyst (0.05 to 0.1 mg cm-2). On the other hand, the methanol oxidation reaction rate is at least three to four orders of magnitude slower on a high Pt-Ru loading (≈ 2 mg cm-2) electrocatalyst. Although thermodynamic
characteristics are similar to the hydrogen reaction, especially in terms of reversible oxidation potential, the methanol electro-oxidation reaction is a slow process and it involves the transfer of six electron to the electrode for a complete oxidation to carbon dioxide.
Thermodynamics of direct methanol fuel cell
Anode reaction: CH3OH + H2O CO2 + 6H+ + 6e- (1)
Cathode reaction: 3/2 O2 + 6H+ + 6e- 3 H2O (2)
Overall reaction: 3/2 O2 + CH3OH CO2 + 2 H2O (3)
The free energy associated with the overall reaction at 25°C and 1 atm and the electromotive force are :
∆G = -686 kJ mol-1
CH3OH; ∆E= 1.18 V (4)
Various reaction intermediates may be formed during the methanol oxidation . Some of these (CO-like) species are irreversibly adsorbed on the surface of the electrocatalyst and severely poison Pt for the occurrence of the overall reaction, which has the effect of significantly reducing the efficiency for fuel consumption and the power density of the fuel cell. Thus, it is vitally important to develop new electrocatalysts to inhibit the poisoning and increase the electro-oxidation rate by at least two-three orders of magnitude. Other species may be released with a consequent decrease of fuel efficiency, whereas, an efficient catalyst must allow a complete oxidation to CO2. Principal by-products in the methanol oxidation are
8 formaldehyde and formic acid. Methyl formiate and other substances have been found in traces.
CH3OH HCHO + 2H+ + 2e- (5)
HCHO HCOOH + 2H+ + 2e- (6) HCOOH CO2 + 2H+ + 2e- (7)
DMFCs are characterized by two slow reactions i.e. methanol electro-oxidation and oxygen reduction with the further drawback of the presence of a mixed potential at the cathode determined by the methanol cross-over. On the other hand, there are specific advantages in using methanol as direct fuel especially for what concerns costs, simplicity of design, large availability, easy handling and distribution. Another concern is that, even though significant progresses have been made in enhancing the electrocatalysis of the four-electron transfer oxygen reduction reaction at low temperatures, the overpotential of this reaction at desired current densities (e.g. 500 mA cm-2) is still about 400 mV in H
2/air fuel cells and increases by
about 50-100 mV in DMFCs because of the effect caused by methanol, which crosses over from the anode to the cathode [3-5].
1.2.1 General comments
In the last few years, a significant amount of investigation has been carried out in the field of electro-oxidation of small organic molecules at low temperature . Most of these fundamental studies have been conducted in half cell configuration and on smooth electrode surfaces, in order to individuate the best electrocatalyst composition . Electrochemical investigations have been generally conducted in combination with spectroscopic techniques in order to elucidate the oxidation mechanism and to investigate the irreversibly adsorbed species on the electrode surface. From a general point of view, almost all electro-oxidation reactions involving low molecular weight organic molecules, such as CO, CH3OH, C2H5OH,
HCOOH, HCHO, require the presence of a Pt-based catalyst [4-8]. A second aspect is that all these electro-oxidation reactions give rise to the formation of strongly adsorbed CO species in linear or bridge-bonded form. Pt is involved in two key steps occurring during the oxidation route. One is the dehydrogenation step (eg. in the case of methanol) and the second one is the chemisorption of CO. Studies involving partial substitution of Pt with other transition metals like W, Pd, Ni, Ti, Rh, Mo have not yielded beneficial results [6-12]. Accordingly, most of the work has been addressed to the modification of the Pt environment by alloying it with
9 other elements or through the synthesis of multifunctional electrocatalysts. The alloying route has given until now the most successful results. It has been shown that the alloying of Sn and Ru with Pt gives rise to electrocatalysts which strongly promote the oxidation of both methanol and CO. Since the complete oxidation of methanol to CO2 involves the transfer of 6
electrons to the electrode, the overall reaction mechanism involves several steps including dehydrogenation, chemisorption of methanolic residues, rearrangement of adsorbed residues, chemisorption of oxygenated species (preferentially on the alloying element) and surface reaction between CO and OH to give rise to CO2.
The concept of realization of multifunctional catalysts ( Ru-Mo, Ru-W, Ru-Sn, Pt-Ru-oxides, Pt-Ru-W-Sn) is based on the need to promote each reaction step through proper elements [13-16]. What is essentially required is the presence of :
1) dehydrogenation sites
2) labile-bonded CO chemisorption sites 3) labile-bonded OH chemisorption sites 4) redox functionalities.
At present, the rate determining step for methanol oxidation at suitable temperatures (T ≈ 90°C ) on Pt-based catalysts is considered to be either the adsorption of OH species at low potentials or the surface reaction between OH and CO chemisorbed on neighbouring sites; at lower temperatures ( T< 60°C ), the dehydrogenation step could also influence the reaction rate . The achievement of significant reaction rates requires the use of highly dispersed metal phase on electrically conductive carbon black support. In this latter system, the preparation procedure of the catalyst strongly influences its performance for methanol oxidation. In the following paragraphs all these aspects are discussed starting from the oxidation mechanism on Pt surface.
1.2.2 Experimental methods
The mechanism of methanol electro-oxidation was elucidated in the last three-four decades by using a variety of experimental procedures [4-8 ]. The electrochemical methods used for such investigation include mainly steady-state galvanostatic polarizations, cyclic voltammetry and electrochemical transients (chronoamperometry, chronopotentiometry) [4-8, 18-23]. Ac-impedance spectroscopy has been used to a less extent . In general electrokinetic parameters i.e. Tafel slopes, activation energies, reaction orders etc., have been derived by galvanostatic steady-state polarizations and linear potential scans in presence of acidic liquid electrolytes in a temperature range from 25 to 80 °C [25-27]. In situ
10 spectroscopic analyses in conjunction with electrochemistry such as FTIR, mass spectrometry XAS etc. [21-22, 28-32] have been demonstrated very useful for the investigation of adsorbed species and for determination of intermediate compounds formed during the oxidation process. Ellipsometry has been particularly used to in-situ investigate the potentials at which water displacement was occurring especially on Pt-Ru surfaces . The experimental techniques and the information acquired from them in relation to methanol oxidation have been reviewed in a few excellent papers [4-8]. Beside these methods, in the recent years additional techniques and/or methodologies of investigation of methanol electro-oxidation have been proposed. Among them, significant interest has arisen around the following procedures:
i) ultra high vacuum preparation of well defined catalyst surfaces for voltammetric analyses ;
ii) in-situ electrochemical crystal microbalance based studies for detection of adsorbed species [34-35];
iii) in-situ viewing of catalysts surfaces during methanol oxidation by scanning tunneling microscopy ;
iv) in-situ electrochemical NMR studies allowing electronic-level description of metallic-shells in nanoparticle catalysts ;
v) in-situ carbon monoxide stripping voltammetry [38-41];
vi) rotating ring disk method with a recast film of catalyst particles/Nafion deposited on an inert glassy carbon electrode to screen electrocatalysts [42-43];
vii) combinatorial methods for the screening of a large variety of catalysts’ formulations .
Some of these techniques are still dealing with smooth electrode surfaces. The acquired information serves mainly to understand the mechanism at a basic level. Yet, there is a need to develop methodologies which allow to get information on the mechanisms occurring at high surface area electrodes and during fuel cell operation. In this regard in-situ CO stripping voltammetry is a very interesting methodology for the characterization of the catalyst / solid polymer electrolyte interface under fuel cell conditions. The information acquired from it regards an evaluation of active surface area, intrinsic catalytic activity and in some cases information on the surface composition of the catalysts is derived . The presence of a close relationship between the anodic shift of the peak potential of the CO stripping and the catalytic activity towards methanol oxidation provides a clear evidence that CO removal is a rate determining step in the methanol electro-oxidation process .
11 A particular importance is played by the combinatorial analysis. This method is addressed to the discovery of new catalyst formulations and it has recently attracted a significant interest . These studies have pointed out the need of a systematic screening of a large number of combination of elements as a suitable route to address the problem of finding better catalysts for methanol oxidation. As a result of these studies Pt-Ru-Os was proposed as one of the most interesting catalyst formulations.
1.2.3 Structural effects and electrode-kinetics
The electrokinetic parameters have been mainly determined at Pt-based electrodes. A Tafel slope between 90 and 120 mV dec-1 was determined for the methanol oxidation reaction at Pt-based catalysts in the temperature range between 25 and 60 °C [15, 22, 29]. This may vary depending on the potential region where it is determined. The Tafel slope in the temperature range from 100 to 130 °C is around 130-140 mV dec-1. If one takes into account
the effect of temperature, the observed Tafel slopes under DMFC operation conditions at high temperatures are very close to those observed in presence of liquid electrolytes at smooth electrodes. A fractional positive reaction order with respect to methanol concentration has been observed in half cell studies in a range of concentrations from 0 to 2.5 M . The Temkin adsorption isotherm has been often used to describe the adsorption of methanolic residues [27, 45, 46] and various kinetic equations describing the variation of current as function of potential, temperature, coverage of adsorbed species have been proposed [46-49]. Bagotzky and Vassilyev derived functional expressions for methanol electrocatalysis at Pt based electrodes for two potential regions characterized by significantly different rates in water discharging i.e. for slow and fast water discharging process on the surfaces . At a fixed potential, the current density (i / mA cm-2) varies with the coverage on the basis of the
i = k ϑOH exp (ϒ1 r1 ϑOrg) (low potentials)
i = k exp (ϒ1 r1 ϑOrg)·exp(ϒ2 r2 ϑOH) (high potentials)
where k is a kinetic constant, ϑOrg and ϑOH are the coverages of methanolic residues and
oxygen species, respectively, ϒ and r are electro-kinetic and Temkin parameters, respectively . These latter take into account the effects of the heterogeneous surface and the interaction between adsorbates. The second relationship holds in the potential region where water displacement and consequent OH chemisorption on the catalyst surface occurs at acceptable rates. For a Pt-Ru surface this region shifts to very low potentials. Although more recent studies have proposed alternative and more complex equations [48, 49], the
12 functional expression proposed by Bagotzky and Vassilyev have been demonstrated useful in interpreting kinetic data for a wide variety of catalyst-electrolyte interfaces. The activation energy for methanol electro-oxidation strictly depends on the catalytic system; Pt-Ru shows activation energy of 30-65 kJ mol-1[25, 26, 50]. Yet, this value is significantly high and it clearly indicates the need of high temperature operation. The exchange current density (Io) for methanol oxidation at various Pt-based catalysts is a few orders of magnitude lower than that of H2 oxidation [2, 51]. Io is obtained by intersection of the Tafel line with reversible
potential for the methanol electrooxidation. As opposite of other electro-catalytic reactions, this parameter is sparely used to quantify the electro-catalyst activity. More often, mass and specific activities at defined potentials, where the reaction is under kinetic control (e.g. 0.25 V - 0.35 V vs. RHE for high temperature operation) are utilized to assess catalysts’ reactivity. This probably depends on the fact that it is not always possible to determine the Tafel slope and/or the Tafel slope changes in the various potential regions [23, 26, 49, 50].
Electro-oxidation of methanol is a structure sensitive reaction. The first studies carried out on Pt surfaces with different crystallographic orientations and for polycristalline Pt evidenced an increased reactivity for methanol oxidation at the Pt planes with (110) Miller indexes  and for rough surfaces [18, 29]. Yet, recently Wieckowski et al. [53, 54] showed for Pt-Ru surfaces that the catalytic activity is maximized by the presence of (111) crystallographic planes. These evidences may be explained by the fact that water displacement at Pt sites occurs very slowly at low electrode potentials. Thus, in the case of a pure Pt catalyst, there is a strong need of Pt sites with high coordination numbers or surfaces with a large number of defects. These sites are capable of chemisorbing oxygen molecules at lower potentials. As opposite, in the Pt-Ru system, the water displacement occur at low potentials on Ru sites whereas methanol chemisorption involves three neighbouring Pt sites. CO removal which is often the r.d.s. at Pt-Ru surfaces  requires the presence of OH species adsorbed on adjacent Ru sites. These latter processes are accelerated by the presence of low Miller index planes. Implications for the development of high surface area catalysts are discussed in a following paragraph.
1.2.4 Pt electrocatalysts
The electrochemical oxidation of methanol on Pt involves several intermediate steps, i.e. dehydrogenation, CO-like species chemisorption, OH (or H2O) species adsorption,
chemical interaction between adsorbed CO and OH compounds, and CO2 evolution. One of
13 particular catalyst surface (crystallographic orientation, presence of defects, etc.). The state of the art electrocatalysts for the electro-oxidation of methanol in fuel cells are generally based on Pt alloys supported on carbon black [6,7,55], even if the use of high surface area unsupported catalysts has recently gained momentum [56, 57]. As stated above, the electrocatalytic activity of Pt is known to be promoted by the presence of a second metal, such as Ru or Sn, acting either as an adatom or a bimetal. The mechanism by which such synergistic promotion of the methanol oxidation reaction is brought about has been the subject of numerous studies during the last 30-40 years, in which various spectroscopic methods have been employed in conjuction with electrochemistry [4-8]. A combination of cyclic voltammetry , in-situ ellipsometry , X-ray absorption spectroscopy , on-line mass spectrometry  and in-situ FTIR spectroscopic studies [22, 28, 29], revealed that the electro-oxidation of methanol on Pt-based catalysts proceeds through the mechanism (sequence of non-elementary reaction steps) below described. First a sequence of dehydrogenation steps give rise to adsorbed methanolic residues, according to the following scheme:
CH3OH + Pt → Pt-CH2OH + H+ + 1 e- (8)
Pt-CH2OH + Pt → Pt-CHOH + H+ + 1 e- (9)
Pt-CHOH + Pt → PtCHO + H+ + 1 e- (10)
A surface rearrangement of the methanol oxidation intermediates gives carbon monoxide, linearly or bridge-bonded to Pt sites, as following:
PtCHO → Pt−C≡O + H+ + 1e- (11a)
PtCHO + Pt → 〉C=O + H+ + 1e- (11b)
In absence of a promoting element, water displacement occurs at high anodic overpotentials on Pt with formation of Pt-OH species at the catalyst surface.
Pt + H2O → PtOH + H+ + 1e- (12)
The final step is the reaction of Pt-OH groups with neighbouring methanolic residues to give carbon dioxide:
PtOH + Pt CO → 2Pt + CO2 + H+ + 1e- (13)
The overall oxidation process of methanol to carbon dioxide proceeds through a six electron donation process; yet, the rate determining step, derived from electrochemical
steady-14 state measurements on Pt, through analysis of the Tafel slope, involves a one-electron step . On a pure Pt surface, the dissociative chemisorption of water on Pt is the rate determining step at potentials below ≈ 0.7 V vs. RHE, i.e. in the potential region that is of technical interest . It is generally accepted that an active catalyst for methanol oxidation should give rise to water displacement at low potentials and to "labile" CO chemisorption. Moreover, a good catalyst for methanol oxidation should also catalyze the oxidation of carbon monoxide.
Even if various theories have been put forward to explain the promoting effect of the additional elements [13, 23, 58, 59], the subject remains controversial. Transition metal promoters and adatoms are seen as a means to improve the electrocatalytic behaviour of electrodes, either by minimizing the poisoning reaction or enhancing the main oxidation reaction. Besides, three main hypotheses have been made. A first hyphothesis suggests that the metal promoters and adatoms either alter the electronic properties of the substrate or act as redox intermediates [59, 60, 61]. This hypothesis, supported by experimental evidences, also leads to the influence of a possible steric effect on the enhanced oxidation rate . A second hypothesis envisages ad-atoms as blocking agents for the poison forming reaction, assumed to occur on a number of sites greater than those required for the main reaction . A third hypothesis based on the bifunctional theory invokes a mechanism by which the oxidation reaction of either the fuel or the poisoning intermediate is enhanced by the adsorption of oxygen or hydroxyl radicals on promoters or adatoms adjacent to the reacting species . Combining the electronic and bifunctional theories it is derived that the role of the second element is to increase the OH adsorption on the catalyst surface, at lower overpotentials, and to decrease the adsorption strength of the poisoning methanolic residues.
1.2.5 Pt-Ru binary alloy electrocatalysts
According to the mechanism shown above it is generally accepted that Pt sites in Pt-Ru alloys are especially involved in both the methanol dehydrogenation step and the strong chemisorption of methanol residues. At suitable electrode potentials (0.2 V vs. RHE), water discharging occurs on Ru sites with formation of Ru-OH groups at the catalyst surface :
Ru + H2O → Ru-OH + H+ + 1e- (14)
The final step is the reaction of Ru-OH groups with neighboring methanolic residues adsorbed on Pt to give carbon dioxide:
15 The chemisorption process of methanol on Ru sites is significantly less favored than on Pt sites, but it is strongly activated by the temperature ; methanol dehydrogenation occurs on Pt at potential values below 0.2 V vs. RHE . Besides, the water displacement reaction, producing oxygen species chemisorbed on Ru sites, occurs at potentials as low as 0.2 V vs. NHE. Although at high temperatures (90 to 130 °C), Ru can participate in the methanol chemisorption process at low potentials, the chemisorption energy of oxygen on Ru surfaces is so high (330 kJ⋅mol-1)  to inhibit Ru sites to be covered by methanolic residues; hence,
they can suitably chemisorb OH groups. The CO removal process is also activated by an increase in temperature and in overpotential .
Although, the argument remains still controversial [17, 23, 34, 35, 43, 64-67], an optimal Ru content in carbon supported Pt-Ru catalysts for the methanol oxidation reaction at high temperature 90-130°C has been found to be 50 at % [68, Chapter II of this thesis]. The optimum Ru surface composition is referable to the relevant synergism accomplished by a Pt-Ru surface with 50% atomic Pt-Ru in maximizing the product of θOH (OH coverage) and k
(intrinsic rate constant), according to the assumption of the surface reaction between COads
and OHads as rds; on the other hand, methanol adsorption and dehydrogenation processes, as
well as water discharging, are considered to be in equilibrium at high temperatures. At low temperatures the situation is somewhat different. Adsorption of methanol on Pt requires an ensemble of three neighbor atoms whereas oxidation of methanolic residues requires a chemical interaction with neighbor adsorbed OH groups on Ru sites. Gasteiger et al.  have observed that methanol oxidation occurs more readily at room temperature on pure Pt-Ru alloys having low Pt-Ru contents (≈ 10%) whereas at intermediate temperatures (60°C) the reaction is faster on alloys with increased Ru contents (≈ 33%). An optimal Ru content in unsupported Pt-Ru catalysts for the methanol oxidation reaction at 130 °C has been found to be about 50 at % . These results can be suitably interpreted by considering that dehydrogenation of methanol is the rate determining step at room temperature. Thus, electrocatalysts having a good fraction of ensembles of three neighbor Pt sites appear to give higher electrochemical activities. At higher temperatures methanol dehydrogenation is thermally activated on Ru sites which participate more actively in the methanol chemisorption process. Under such conditions, the rate controlling steps become the water displacement on Ru sites and the chemical interaction between adsorbed methanolic residues and OH groups. Analysis of specific and mass activity of unsupported Pt-Ru catalysts with different composition at high temperature (130 °C) in a DMFC  indicates the presence of a maximum for a 1:1 Pt-Ru atomic ratio.
16 The synergistic promotion exerted by Pt-Ru alloys is supported by X-ray absorption analysis . Accordingly, an increase of Pt d-band vacancies is produced by alloying with Ru; this possibly modifies the adsorption energy of methanolic residues on Pt. Such evidences suggest that the reaction rate is not only dictated by the bifunctional mechanism but it is also influenced by electronic effects occurring on account of the interaction between Pt and Ru [59-60]. These aspects are discussed more in detail in the next paragraph.
The achievement of significant reaction rates for the Pt-Ru system requires the use of highly dispersed metal phase on electrically conductive carbon black support. In this latter system, the preparation procedure of the electrocatalyst was found to strongly influence its performance for methanol oxidation [4, 43]. Following various studies carried out in this field, the starting point for the development of an active electrocatalyst for CH3OH oxidation
is to synthesize a suitable highly dispersed Pt-Ru phase. A few authors have pointed out the need to develop multifunctional catalysts, thus, often the Pt-Ru system is modified with the addition of a third functionality (Pt-Ru-Mo , Pt-Ru-W , Pt-Ru-Sn [14, 52], Pt-Ru-Os ).
1.2.6 Promoting effects of Ru and Sn: bifunctional mechanism and ligand effect
Both Pt-Ru and Pt-Sn systems have been reported to be promising catalysts for electro-oxidation of methanol in direct methanol fuel cells [8, 52, 70]. But although there is conclusive evidence on catalytic promotion of methanol electro-oxidation on the Pt-Ru system in relation to Pt, contradictory results have been reported in the literature on the promotional effect of tin for this reaction [13, 19, 71-73]. While Janssen and Moolhuysen  and Motoo et al.  have found a 50-100 times enhancement in the electrocatalytic activity of smooth and electrodeposited Pt electrodes on which Sn was deposited, several other authors [71, 72] have reported considerably smaller and even negative effects. For carbon-supported Pt-Sn electrodes, different methods of preparation are found to exhibit varying effects [74, 75] leading to different Pt-Sn surface properties. The surface characteristics of Pt-Ru and Pt-Sn are of considerable significance for the methanol-oxidation reaction. Since both Pt-Ru and Pt-Sn systems have been reported to promote electro-oxidation of methanol, different electronic environments around Pt-sites in Pt-Ru and Pt-Sn should imply different routes for methanol-oxidation reaction. As stated above, the most agreeable mechanism for methanol oxidation on Pt-alloys is based on the bifunctional theory . According to this theory, Pt-sites adsorb methanol through a dehydrogenation step whereas the alloying element, namely Ru or Sn, adsorbs oxygenated species from water. The
17 methanolic residues adsorbed on Pt-sites react with the oxygenated species present on the neighbouring Ru or Sn sites in the alloy producing CO2.
In a previous study , it was observed a 1.1 eV shift in the X-ray near edge spectrum (XANES) of the Pt-Sn/C catalyst with respect to the Pt/C catalyst, from which result one may infer that Sn atoms in the Pt-Sn alloy donate electrons to Pt-atoms and are thereby oxidized. This is in agreement with the electronegativity values for elemental Pt and Sn which differ appreciably. A noticeable charge transfer from Sn to Pt has been also found in an XPS analysis, as reflected by a negative shift in the Pt-4f binding energies of the Pt-Sn samples in relation to Pt/C electrocatalysts .
Recently, Mukerjee and McBreen [59, 77] have shown in their X-ray absorption spectroscopic studies on Pt-Ru/C and Pt-Sn/C electrocatalysts that alloying Sn with Pt causes partial filling of Pt 5d-bands and a consequent increase in the Pt-Pt bond distances with a contrary effect observed for Pt-Ru catalysts. However in other investigations, XPS data on Pt-Ru/C samples have not shown any evidence of modification in the Pt-4f spectra as compared with that in Pt/C samples, which showed consistently nearly the similar electronegativity values for elemental Pt (2.2) and Ru (2.1). Beside the work of Mukerjee and McBreen , some in situ experiments have also provided evidence for the influence of Ru on the electronic state of Pt . Iwasita et al.  observed in their FTIR experiments a shift towards higher frequencies for the CO stretching on Pt-Ru with respect to Pt. This effect has been attributed to a lower chemisorption energy for CO on the Pt-Ru alloy. Frelink et al. [34, 35] measured the stretching frequency of linearly bonded CO as a function of coverage for the Pt and Pt-Ru electrodes. A shift to higher frequencies at various coverages was observed as a result of change in the CO binding strength to the surface induced by Ru through a ligand effect on Pt [34-35]. But, these authors have also shown by in-situ ellipsometric studies on Pt and Pt-Ru electrodes that the Ru-oxide film is removed by reaction with methanol during its electro-oxidation. This evidence supports the bifunctional mechanism. The latter findings were further corroborated by DEMS studies [34, 35]. In a recent article, Iwasita and co-workers have emphasized the bifunctional mechanism for methanol electro-oxidation on the Pt-Ru system . In our opinion, it may be rationalized from the in-situ experiments described above that the promotional effect of Ru could be due to both the contribution of bifunctional and ligand effects. But, the ligand effect in the Pt-Ru system appears to be significantly less prominent and it has still not found support in the results obtained from a few surface techniques including XPS .
18 Further insight on the mechanism can be obtained by analysing the Pt-carbon monoxide bonding since CO removal from Pt surfaces plays a dominant role in methanol oxidation The nature of Pt-CO bond in platinum systems has been well documented in the literature . It would, however, be in context to elucidate the nature of bonds formed between CO and Pt as well as between OH and Ru ( or Sn ) in the respective alloy systems. Chemisorption of CO on Pt involves donation of an electron pair from σ* anti-bonding orbitals of CO to the unfilled 5d-orbitals of Pt. A back donation of electrons from the Pt metal to CO-orbitals further stabilizes their interaction. Accordingly, it is apparent that the dative electron donation from CO to Pt is a pre-requisite for a strong CO-chemisorption. If the Pt surface is partially oxidised, the Pt metal can more easily accommodate the electrons donated by CO in its unfilled orbitals. The increase in the Pt 5d-band vacancies produced by Ru atoms as interpreted by Mukerjee and McBreen , would imply an increase in Pt-CO bond strength which in effect would retard the methanol-oxidation reaction. On this basis, the promoting action of Ru arises mainly due to an easier chemisorption of oxygen from water at lower electrode potentials in accordance with the bifunctional theory. Nevertheless, some modifications of the electronic environment around Pt may occur during the interface formation, since the uptake of oxygen functionalities from water could modify the electron accepting characteristics of Ru atoms. On the other hand, a charge transfer from Sn to Pt in the Pt-Sn system, evidenced from XAS and XPS data, causes a substantial increase in electron density around Pt-sites resulting in a weaker chemisorption of CO. This combined with an easier adsorption of OH-species on the oxidized Sn-sites at lower electrode potentials would enhance the oxidation of irreversibly adsorbed CO to CO2, and would thus promote the
methanol-oxidation reaction. The electro-catalytic promotion of CO electro-oxidation on Pt-Sn alloy at low electrode potentials has been recently discussed by Markovic’ et al. . Accordingly, the Pt3Sn bulk alloy was found significantly more active than the Pt-Ru system
for CO oxidation. However, higher electrode potentials produce a negative effect due to strong adsorption of OH-species on Sn-sites and retard the methanol-oxidation reaction on Pt-Sn catalysts. In many cases formation of stable tin-oxide species on the surface during catalyst preparation or electrode activation procedures has been observed . The presence of these compounds present on the electrode surface play a significant role during the methanol oxidation reaction since the electrocatalyst is operated in a potential regime in which oxide must not be present but where the supply of active oxygen is important. Formation of labile-bonded oxygen species more easily occurs on an oxide-free surface and in this context the water displacement reaction occurs more easily on Ru than Sn sites. Generally, the
19 achievement of properly reduced Pt-Sn surfaces is brought about with difficulty. In this context, Pt surface containing Sn ad-atoms often perform better than bulk or carbon supported Pt-Sn alloy catalysts .
From all these evidences, one may conclude that the addition of Ru to Pt markedly increases the electrocatalytic activity of Pt through the adsorption of oxygenated species on Ru-sites. By contrast, the promotion of CO oxidation reaction on Pt-Sn catalyst appears to be mainly due to a modification of the electronic environment around Pt-sites. It becomes clear that Pt-Ru catalysts are more effective for methanol oxidation since the reaction desires the electrocatalyst to be operated in a potential regime where labile-bonded oxygen should be present on the surface. In this situation, the supply of active oxygen to the surface is of paramount importance since this apparently would facilitate the oxidation of adsorbed methanolic residues to CO2. The presence of strongly-bonded oxygen species on Sn-sites in
the Pt-Sn system limits the oxidation of methanol to CO2.
1.2.7 Role of Ru-oxide in enhancing kinetics
Some Pt-Ru catalysts show a lower Ru content in the Pt-Ru alloy (as detected by XRD) with respect to the nominal composition [57, 81]. In such cases, the remaining Ru atoms are present as RuOx species that may be composed of crystalline tetragonal RuO2 or amorphous
Ru-oxide [57, 81, 82]. The oxide species are generally detected by XRD or TEM if they have a crystalline structure (frequently RuO2 tetragonal), whereas X-ray absorption spectroscopy
(both EXAFS and XANES) and in some cases XPS may give information on the amorphous Ru-oxide species. Often, TEM micrographs of the carbon supported Pt-Ru sample show some agglomeration of particles having similar dimension but characterized by a different atomic contrast . The interlayer spacing of Pt-Ru alloy particles that may be observed at high magnification is about 2.25-2 Å, corresponding to the (111) planes of the Pt or Pt-Ru fcc lattice. The largest interlayer spacing of the RuO2 structure is 3.17 Å and is
comparable to the interlayer spacing d (002) of the graphitic carbon support but they cannot be confused since the carbon lattice is quite irregular like in an amorphous material and is continuous. Amorphous Ru-oxide particles of small size also can not be easily distinguished. In such case XAS and XPS analyses may indicate the presence of amorphous Ru-oxide; it must be noted that XPS gives information only on the outermost layers . It was reported that formation of labile oxygen groups on Ru sites, not directly alloyed with Pt but close enough to Pt sites, can allow chemical interaction between these groups and the adsorbed methanolic residues to produce CO2. The promoting effect of the RuOx species
20 for methanol oxidation reaction has been extensively investigated by several authors [83-85]; recently, very high performances were obtained in a DMFC with unsupported Pt-RuOx anode
electrocatalyst . It was suggested that facile oxygen transfer from Ru to Pt rich regions where adsorption of CO-like residues preferentially occurs, could enhance the catalytic oxidation of methanol . But, oxygenated species, strongly held on Ru surfaces, cannot easily migrate on the surface. In general XPS analysis has revealed the presence of Ru(IV) and Ru(VI) species. The oxygen transfer mechanism requires an open oxy-hydroxide structure with a significant number of free Ru-OH bonds . Thus, such mechanism operates better on Ru(IV) that on Ru(VI) species since the formation of labile oxygen bonds occurs preferentially on the first sites. It is thought that both mechanisms involving Pt-Ru alloys and RuOx species could actively participate in the methanol oxidation reaction.
Yet, the absence of an atomic mixing of Pt with RuOx species probably imposes an
activation barrier for the migration of adsorbed intermediates. In order to assess which mechanism is more effective, in a recent study the methanol oxidation behaviour on a pure Pt-Ru alloy and a Pt-RuOx electrocatalyst, with comparable particle sizes, have been compared at high temperatures (130 °C) [84, 86, Chapter II of this thesis]. It was observed that both electrocatalysts are active for the methanol oxidation reaction but the electrocatalyst containing a lower amount of oxidized Ru species and characterized by a smaller Ru-O bond strength performed better [84, 86].
1.2.8 Ternary alloy Pt-Ru-W and Pt-Ru-Mo electrocatalysts
The Pt-Ru formulation suffers the lack of other elements able to promote a “labile” adsorption of carbon monoxide-like species and /or to oxidize these methanolic species by an effective redox mechanism. In this light, an interesting approach is the formulation of new electrocatalysts that, although based on Pt-Ru alloy (this has demonstrated irreplaceable characteristics in matching the above requirements), would take advantage of proper surface promoters able to facilitate labile adsorption of methanol residues and their oxidation through redox functionalities. In recent years, electrocatalyst formulations which includes tungsten and molybdenum have been proposed [2, 14, 69, 87]. In an acid electrolyte environment, these elements are generally stable in one or more oxidized forms such as WO2/WO3 or
WO2/WO3 and can easily exchange oxidation states by adsorbing hydroxyl ions from water
and donate these species to methanol residues adsorbed on Pt. Recently, Tseung et al.  have shown that the Pt-Ru-W system shows superior electrocatalytic activity, if W is present in a reduced form, for CO oxidation. Similar evidences were found for the ternary system
21 containing molybdenum . But in this latter system, the electrochemical stability of molybdenum, under prolonged operation conditions, has still not been demonstrated.
Tungsten has the ability of coordinating water and a high mobility of hydroxyl species in the WO3/WO2 system in the region near the reversible potential for the oxidation of
methanol, i.e. 0.04 V vs. NHE. The formation of hydrogen tungsten bronze, HxWO3, during
the dehydrogenation process of methanol was observed for Pt/WO3 electrocatalysts . The
presence of a “spillover” effect has a significant influence on the activity of the catalysts. Tungsten oxide-containing electrocatalysts produce an enhancement of the reaction rate by the continuous formation and oxidation of HxWO3 during the dehydrogenation of methanol.
Furthermore, water is adsorbed on WO3 at low overpotentials and may interact with CO
adsorbed on Pt, thus facilitating its oxidation to CO2.
Polyfunctionality is thought to be a prerequisite for oxidation of methanol, since it involves a series of intermediate steps. Whilst CO chemisorption is affected by the electronic environment and will be governed by the electron accepting-donating characteristics of Ru and W on Pt, including the promoting effect on the water discharge reaction at low potentials, the dehydrogenation process requires Pt with the added benefit of a significant spillover. The development of an active multifunctional catalyst, combining a redox functionality to the dehydrogenation step on Pt sites and the dehydroxylation step on Ru sites, is expected to constitute a fundamental “breakthrough” for DMFCs.
1.2.9 Heteropolyacids as surface promoters
A parallel strategy to the development of a new electrocatalyst for methanol electro-oxidation would be to employ co-catalysts or catalytic enhancers; accordingly, heteropolyacids have been demonstrated to be potential candidates in this approach [63, 89]. In the last few years, research on heteropolyacids has been a topic of remarkable and widespreading technological interest. The source of this interest mainly lies upon their unique structural and chemical characteristics, as well as on their capacity to exert various catalytic functions. In a previous study, it was shown that the electro-oxidation of methanol is promoted by an heteropolyacid, i.e. silicotungstic acid, but not by other inorganic acidic electrolytes, such as sulfuric acid . More recently, other authors have shown that the enhancing behaviour of H4SiW12O40 for methanol electro-oxidation is still present even when
the heteropolyacid is dissolved in small amounts in sulfuric acid . The observed improvements in the methanol oxidation activity in the presence of H4SiW12O40 may be due
22 those of methanol adsorption, which thereby promotes the oxidation of strongly adsorbed methanolic residues. These results were supported by the improved kinetics of the electro-oxidation of carbon monoxide in phosphotungstic acid (PWA) electrolyte  over that in sulfuric acid. In particular, PWA was proven to enhance the water discharging process and the oxidation of CO species strongly bonded to the Pt electrocatalyst . Heteropolyacids have also been used as surface promoters for another irreversible, electrochemical reaction (the oxygen reduction) when used as aqueous liquid electrolytes . Recently, it was shown that heteropolyacids can be suitably anchored on active carbon supports and used as catalysts in heterogeneous oxidation reactions . Tungstic acid (H2WO4) has been employed as a
catalytic enhancer of Pt in phosphoric acid fuel cells by a simple blending procedure during electrode preparation . Such evidences suggest that a novel route to increase the overall reaction rate may be based on the use of heteropoly-metallates as substrate species in conjunction with Pt-Ru catalysts.
1.2.10 Alternative electrocatalysts to platinum and their alloys
Only a few electrocatalyst formulations, alternative to Pt, have been proposed for methanol electro-oxidation. In most cases, the alternatives contain noble metals like gold, which does not solve the problem of the high cost of the materials employed in DMFCs. Only, a few formulations without noble metals have been tested: these are mainly based on transition metal alloys like NiZr , transition metal oxides and tungsten based compounds [9,10, 94]. All these materials showed lower reaction rates than Pt-based electrocatalyst and thus such unsatisfactory preliminary results have not stimulated much work in these directions.
Although many studies have been directed to the investigation and optimization of noble metals electrocatalysts, little work has been devoted to explore the possibility of using transition metal oxides as anodes. Transition metal oxides can play a role through their electron accepting and donating sites on the surface, and thereby adsorb methanol and CO related species. As an example, an oxidation mechanism, already proposed in gas-phase heterogeneous catalysis , is as follows:
(16) Transition metal oxides, because of their partially filled orbitals, may be ideal for a labile interaction with carbon monoxide and also be able to chemisorb hydroxyl species on neighbour sites. So far, the investigation of transition metals and metal oxide as electrocatalysts in DMFCs has been hampered by the corrosive characteristics of sulfuric and phosphoric acid electrolytes. However, the promising performance characteristics of DMFCs based on solid polymer electrolytes stimulate a reconsideration of non stoichiometric metal oxides, in view of their ability to oxidize water at low potentials, which is an essential feature for methanol oxidation. As transition metal oxide compounds intrinsically possess the thermodynamic characteristics which predict water displacement at low overpotentials, one could expect that, their wide range of potential for electro-reduction might meet the demand for the essential reaction through a surface oxygen vacancy mechanism.
In the following, a scheme of the thermodynamic potentials (E°) for the interaction of water with a few transition metal/metal oxides is presented and compared to that on Pt :
Pt + H2O → PtO + 2H+ + 2e- E° = 0.99 (17) Mo + 3H2O → MoO3 + 6H+ + 6e- E° = 0.25 (18) W + 2 H2O → WO2 + 4H+ + 4e- E° = - 0.05 (19) W + 3H2O → WO3 + 6H+ + 6e- E° = 0.09 (20)
The considerable lower values of E° for the Mo/MoOx and W/WOx redox complexes than that for the Pt/PtO one, enhances the ability of coordinating water (at any significant concentration) by the metallic site and generating mobile hydroxyl species. As the most favourable condition for water displacement occurs in the region near to the reversible potential for oxidation of methanol, i.e. 0.04 V vs. RHE, transition metals like Mo and W appear ideally suitable for accelerating the rate of methanol oxidation. In particular, tungsten oxides show similar behaviour at different oxidation states. The doping of tungsten oxide with
24 rare earth elements or Na-alkali increases the rate of oxidation of pure carbon monoxide and of CO in reformed gas in a fuel cell . This will open favourable perspectives, depending upon the degree of reduction of the bronzes, and whether water chemisorption can be tuned and the OH mobility adjusted through regulation of density of oxygen vacancies. Beside tungsten oxides, tungsten carbide is also known to possess intrinsic catalytic activity for electro-oxidation reactions such as hydrogen oxidation . Although WO2 was demonstrated
to be very active for CO oxidation in a fuel cell as early as 1969 , it has only recently been shown that tungsten oxides and bronzes also have electrocatalytic activity for this reaction as well as methanol oxidation . Furthermore, the concentration of oxygen vacancies on the electrocatalyst surface of tungsten bronzes can be appropriately adjusted by the addition of sodium or rare earth elements, so as to attain the desired range of potential for oxidative removal of the adsorbed CO by the active species generated on the surface of the electrocatalyst [97, 98]. According to the premises, the development of an active multifunctional catalyst, combining the dehydrogenation step promoted by tungsten carbide with a dehydroxylation step on the transition metal oxide site, may constitute the required "breakthrough" required for the reduction of noble metal loading in the anode and for further progress to make DMFCs commercially viable.
I.2.1.3 Morphological aspects of electrocatalysts
1.3.1 Role of surface area and metal loading
As discussed above, the main requirement for an optimal alloy electrocatalyst, such as Pt-Ru, is to synthesize it, highly dispersed on a carbon support. The mass activity (A/g Pt) of the catalyst for methanol electro-oxidation is strictly related to the degree of dispersion, since the reaction rate is generally proportional to its active surface area. In the case of an oxygen reduction electrocatalyst, it was found, after analysing a wide range of Pt and Pt alloy electrocatalysts, that there is an optimum particle size for the metallic phase (about 30 Å), which corresponds to a significantly high mass activity . For this reaction it was found that the specific activity (mA cm-2 real surface area) increases with the particle size, but simultaneously decreases with the active surface area. The best compromise was achieved at about 30 Å Pt particle size .
In the case of methanol electro-oxidation on carbon supported Pt electrocatalyst, two different trends were observed. Mc Nicol et al.  observed for their Pt electrocatalysts a maximum activity at about 80 m2/g surface area. Recently, another group has shown that the
25 specific activity increases as a function of particle size . Thus, a maximum in mass activity vs. particle size should be observed as in the case of oxygen reduction. On the other hand, Watanabe et al.  found that the specific activity for methanol oxidation on a carbon supported Pt electrocatalyst does not change for a particle size above 20 Å (Pt fcc structure); thus, the mass activity increases as the dispersion of the metal phase is increased . These latter findings have been in part confirmed for the Pt-Ru system for a particle sizes above 30 Å . Not much work has been carried out on electrocatalysts with particle sizes below 20 Å or catalyst formed by an amorphous phase. Generally, most of the Pt-Ru fuel cell electrocatalysts have particle sizes above 20 Å, which are crystalline with a face centered cubic (fcc) structure. Below 20 Å, the distinction between amorphous and crystalline is not so evident. For particles with 10-15 Å size about 50% of the atoms are on the surface and thus there is no ordered structure. Some recent kinetic investigations by Wieckoski et al. [53, 54] on Pt surfaces covered with Ru ad-atoms have shown that the surface composed by the (111) Pt crystallographic plane covered by Ru atoms performs better than any other Pt/Ru ad-atoms crystallographic plane. Thus extending these considerations to high surface area Pt-Ru electrocatalysts, the specific activity should increase with the particle size. In fact, a large-size particle possess a high surface content of (111) planes . Accordingly, a maximum in the electrocatalytic activity should be observed as a function of particle size. In effect the data shown by Ren et al.  may be fitted as well with a “volcano” relationship with maximum at 3 nm and shape similar to that generally observed for oxygen reduction. Unfortunately, the scattering due to a variable composition of the Pt-Ru surface, in high surface area electrocatalysts, does not allow to distinguish a clear behaviour. A second aspect concerns the loading of the metal phase on the carbon support. A high wt. percent of Pt on the carbon substrate will significantly decrease the anode thickness for the same Pt loading per geometric electrode area (eg. 1 mg cm2). Using this approach, it will be possible to enhance mass transport through the electrode and simultaneously reduce the ohmic drop. However, it has been found that an increase of the Pt loading (above 40 % wt.) on the carbon support decreases the dispersion of the electrocatalyst, probably due to some particle agglomeration.
1.3.2 Role of carbon support
In general preparation procedures, such as impregnation, colloidal deposition, surface reaction involve the adsorption step of active compounds on a carbon black surface. The synthesis of a highly dispersed electrocatalyst phase in conjuction with a high metal loading on carbon support has been one of the goals of the recent activity in the field of DMFCs. In
26 this regard it is of interest to determine which carbon black is most suitable as the support. In recent reports [103- 105], the mostly used carbon blacks were: Acetylene Black (BET Area: 50 m2/g), Vulcan XC-72 (BET Area: 250 m2/g) and KETJEN Black (BET Area: 1000 m2/g).
All these materials have optimal electronic conductivity but, as denoted above, they differ for the BET surface area and thus very probably in the morphology. A low surface area carbon black (such as Acetylene Black) will not allow high dispersion of the metal phase, especially for a high metal loading (low carbon content); on the other hand, it does not have micropores in the structure, which could hinder mass transport through the electrocatalytic layer. A high surface area carbon black can easily accommodate a high amount of metal phase, with a high degree of dispersion but, at the same time, the significant amount of micropores on the carbon support will not allow a homogeneous distribution of the electrocatalytic phase through the support, which could lead to mass transport limitations of the reactant as well as its limited access to the inner electrocatalytic sites. Vulcan XC appears to be the best compromise with the presence of a small amount of micropores and a reasonable high surface area sufficient to accommodate a high loading of the metal phase. Up to now, this carbon black is the most used carbon support for the preparation of DMFCs catalysts.
1.3.3 Preparation methods
There are various routes for the synthesis of the Pt-Ru/carbon black electrocatalyst; these can be grouped into two main type, i.e., impregnation and a colloidal procedure. An impregnation procedure is characterized by an impregnation step of Pt and Ru precursors (e.g. H2PtCl6, Ru Cl3, Pt(NH3)2(OH)2, Ru3CO12, Pt(NH3)2(NO)2 etc.) which is followed by a final
reduction step. This can be a chemical reduction of the electrocatalyst slurry in aqueous solution by using N2H4, NaS2O5, NaS2O3, NaBH4 (liquid-phase-reduction) or gas-phase
reduction of the impregnated carbon black by a flowing hydrogen stream. It has been shown that the impregnation method can be used for the synthesis of a multifunctional system, e.g. from a bimetallic to a quaternary electrocatalyst (Pt-Ru-Sn-W) . However, it requires the use of high surface area carbon black such as Ketjen black whose limitations for the operation of a methanol fuel cell have been pointed out above. Furthermore, this procedure does not allow one to obtain high dispersions in presence of high metal loadings.
There are various colloidal deposition routes, as, for example, used by Jalan , Bonneman et al. , Petrow and Allen , etc. The advantages of these preparation
27 routes consist in the attainment of significantly high surface areas in the presence of high metal loading on carbon. The main disadvantages are the presence of some complex preparation steps in the overall synthesis, the use in some cases of organic compounds/solvents and the increase of costs of production. An additional method is based on the thermal decomposition. In this case unsupported high surface area electrocatalysts are obtained by thermal decomposition of appropriate high molecular weight Pt-precursors such as Pt-carbonyl compounds . Other methods, such as co-precipitation sol-gel or physical methods (e.g., sputtering ) have not stimulated much interest in the past but they are now becoming interesting for the synthesis of catalysts for portable power sources . The choice of the most appropriate preparation procedure relies on the following considerations. It is well known that the preparation procedure of electrocatalysts influences their physico-chemical properties and thus their activity for methanol oxidation reaction and the oxygen reduction. The performance characteristics of an electrocatalyst depend on its chemical composition (surface and bulk), structure and morphology. Accordingly, the selected methodology of electrocatalyst synthesis should allow one to address the process for the attainment of a proper structure (crystalline or amorphous) and with a chemical composition on the surface as close as possible to the nominal or bulk composition. Since the rate of all electrocatalytic reactions is strictly related to the active surface area besides surface chemistry, the morphology of the electrocatalyst needs to be tailored. Morphology is not only related to the metal-phase area but also to the presence of micro and macro pores in the electrocatalyst support which could facilitate or hinder the mass transport properties. All these characteristics determine the cell performance even if the relative influence of each parameter is still not known in detail. It is thus necessary to select appropriate procedures for an optimization of these characteristics i.e. composition, structure, particle size, porosity etc. Generally a combination of physico-chemical and electrochemical analyses carried out on electrocatalysts with different characteristics indicates the system that better suits the scope of application in a DMFC.
I.2.2 Cathodic reduction of oxygen
2.1 General considerations
Although Pt/C electrocatalysts are, at present, the most widely used materials as cathodes in low temperature fuel cells, due to their intrinsic activity and stability in acidic solutions, there is still great enthusiasm to develop more active, selective and less expensive
28 electrocatalysts for oxygen reduction. Since it is widely established that Pt cannot be easily replaced (at least for the moment) by other electrocatalysts for the oxygen reduction reaction (ORR), there are a few directions that can be investigated to reduce the costs and to improve the electrocatalytic activity, especially in the presence of methanol cross-over. One is to increase Pt utilization. This can be achieved either by increasing its dispersion on carbon and the interfacial region with the electrolyte. Another successful approach to enhance the electrocatalysis of O2 reduction is by alloying of Pt with transition metals. This enhancement
in electrocatalytic activity has been differently interpreted, and several studies were made to analyze in depth the surface properties of the proposed alloys combinations [111-115]. Although a comprehensive understanding of the numerous reported evidences has not yet been reached, the observed electrocatalytic effects have been ascribed to several factors (interatomic spacing, preferred orientation, electronic interactions) which play, under fuel cell conditions, a favourable role in enhancing the ORR rate [116-120]. High specific activities of Pt-Cr and Pt-Cr-Co alloy electrocatalysts for oxygen reduction as compared with that on platinum were observed in H2-air polymer electrolyte membrane fuel cells
(PEMFCs) [111,120]. The formation of a tetragonal ordered structure upon thermal treatment, in the case Pt-Co-Cr, leads to a more active electrocatalyst than that with a Pt fcc structure [116-120]. Moreover, even in the presence of methanol cross-over, the performance of highly selective electrocatalysts for oxygen reduction would be (in theory) less affected by poisoning phenomena on account of the lower chemisorption energy of methanol on the alloys in comparison with that on Pt. Another goal in this field is to obtain very small sizes for the Pt alloy particles supported on carbon. In the case of Pt-Co-Cr particles with a tetragonal structure, the state of art electrocatalysts have a particle size of 6 nm [116-120]. In addition to the coprecipitation and impregnation methods for preparation of these alloys on a carbon support, colloidal preparation procedures have also been recently investigated .
2.2 Oxygen electroreduction in DMFCs
For the development of cathode electrocatalysts for DMFCs, two main aspects should be taken into account. The electrocatalysts should be very selective for oxygen chemisorption and thus highly active for oxygen electroreduction. In other words, the electrocatalysts should have a composition which will not be poisoned by the methanol crossing over from anode to cathode while maintaining high reaction rates for oxygen reduction. In most cases, a compromise between electrocatalytic activity and resistance to poisoning is necessary. The
29 most widely used electrocatalysts employed in low temperature fuel cells for the oxygen reduction are based on platinum. As discussed in a previous section, various studies conducted in the past, especially on carbon supported Pt electrocatalysts for oxygen reduction in phosphoric acid fuel cells, showed that the electrocatalytic activity (mass activity, mA g-1 Pt, and specific activity, mA cm-2 Pt) depends on the mean particle size. The mass activity for oxygen reduction reaches a maximum at a mean particle size of 30 Å, corresponding closely to the particle size at which there is a maximum in the fraction of (111) and (100) surface atoms on Pt particles of cubo-octahedral geometry . On the other hand, the specific activity increases gradually with an increase in the Pt particle size and closely follows the trend observed between the surface fraction of (111) and (100) Pt atoms and the particle size. These results have indicated that the (111) and (100) surface atoms are more electro-catalytically active than Pt atoms located on high Miller index planes . Platinum atoms at edge and corner sites are considered to be less active than Pt atoms on the crystal faces. Accordingly, the mass and specific activity should decrease significantly as the relative fraction of atoms at edge and corner sites approach unity . This situation occurs with Pt particles smaller than 10 Å diameter. Most of the experimental evidence observed in PEMFCs, shows that crystalline electrocatalysts with about 25-30 Å particle size have higher activities than amorphous particles and also electrocatalysts with larger crystallite sizes .
In the case of DMFCs, an additional aspect should be considered; this is in regard to the methanol cross-over through the membrane. Methanol oxidation and oxygen reduction in the cathode compartment compete for the same sites producing a mixed potential which reduces the cell open circuit potential. In order to better understand these effects, it is worthwhile considering the mechanism for methanol oxidation and oxygen reduction; possible mechanisms are presented below.
O2 + Pt → Pt-O2 (21)
Pt-O2+H++1e- → Pt-HO2 (22)
Pt-HO2+Pt ⎯ →⎯ Pt-OH+Pt-O rds (23)
Pt-OH+Pt-O+3H++3e- →2Pt+2 H2O (24)
Equation (23) indicates an intermediate step requiring a dual-site reaction, and if it is the rate-determining step, it is more affected by particle size than intermediate step represented by equation (22). When the particle size becomes very small, then only the inactive edge and corner atoms will be present and dual sites of the proper orientation would not be available. Thus the activity of the particle should be lower. According to the observed variation of the
30 reaction rate with particle size, one may conclude that the rate-determining step is represented by Eq. 23 . Methanol oxidation: CH3OH+3Pt → Pt3-COH (25) Pt3COH → Pt-CO+H++2Pt (26) Pt+H2O → Pt-OH+H++1e (27) Pt-OH+PtCO → 2Pt+CO2 (28)
In the case of methanol oxidation at the cathode, three neighboring Pt sites in a proper crystallographic arrangement will favour the methanol chemisorption. Since at high cathodic potentials the water discharging reaction (eq. 27) is largely favoured, oxidation of the methanolic residues adsorbed on the surface proceeds very fast producing a parasitic anodic current on this electrode.
When the particle size of the electrocatalyst is very small or one has an amorphous Pt electrocatalyst for the oxygen reduction, methanol chemisorption energy could be lower and hence the cathode less poisonable. But, at the same time, due to the fact that only the inactive edge and corner atoms will be present and dual sites of the proper orientation will not be available, the activity of such electrocatalyst for oxygen reduction will be lower. The best compromise is to modulate the structure and the particle size between amorphous and crystalline in order to decrease the poisoning by methanol and enhance oxygen reduction. A second possibility is to use a promoting element for oxygen reduction which simultaneously hinders the methanol chemisorption still maintaining the proper structure and particle size.
2.3 Carbon supported electrocatalysts
In order to enhance the resistance to methanol poisoning of the cathode, research activities based on the modification of Pt electrocatalyst by addition of transition metals were recently initiated in various laboratories [121, 123]. In phosphoric acid and PEMFCs the intrinsic electrocatalytic activity of Pt alloys (Pt-Cr, Pt-Ni, Pt-Cr, Pt-Cu, Pt-Fe), with a lattice parameter smaller than that of Pt, is higher than on the base metal [111-120]. This effect is related to the nearest neighbour distance of Pt-Pt atoms on the surface of the fcc crystals. Since it has already been observed that the rate determining step involves the rupture of the O-O bond through a dual site mechanism, a decrease of the Pt-Pt distance favours the dual site O2 adsorption. Most of these evidences are derived from studies carried out in phosphoric acid